- Home
- Documents
- Bridging Gaps in Laser Transmission Welding of vandeven/JournalPaper-Bridging Gaps in LTW.pdfchanges in process parameters necessary to bridge a gap within reasonable welding velocities and can be easily constructed with commercially available shims.Published in: Journal of Manufacturing Science and Engineering-transactions of The Authors: James D Van De Ven Arthur G ErdmanAffiliation: University of MinnesotaAbout: Laser beam welding Welding Process control Engineering design

Published on

24-Mar-2018View

214Download

2

Embed Size (px)

Transcript

B

jedlccg

dfpcbtbttwp

Leic1i

iNL

J

Downlo

James D. Van de Vene-mail: vandeven@me.umn.edu

Arthur G. Erdmane-mail: agerdman@me.umn.edu

Mechanical Engineering Department,University of Minnesota,

111 Church Street Southeast,Minneapolis, MN 55455

Bridging Gaps in LaserTransmission Welding ofThermoplasticsGaps at part interfaces pose a major challenge for laser transmission welding (LTW) ofthermoplastics due to the reliance on contact conduction between the absorptive andtransmissive parts. In industrial applications, gaps between parts can occur for a varietyof tolerance and process control reasons. Previous experimental and modeling work inLTW has focused on gap-free joints, with little attention to bridging a gap with thermalexpansion of the absorbing material. A two-dimensional comprehensive numerical modelsimulated bridging gaps in LTW. Using the model, operating parameters were selectedfor welding across a 12.7 m gap and a 25.4 m gap by creating sufficient thermalstrain to bridge the gap and form a weld. Using these operating parameters, PVCsamples were welded in a T-joint geometry with a designed gap. The quality of the weldswas assessed visually, by destructive force testing and by measuring the weld size toquantify the weld strength. All the experimental samples, for the two gap sizes, bridgedthe gap and formed welds. The average weld strength of the 12.7 m gap samples was16.1 MPa, while the 25.4 m gap samples had an average strength of 10.0 MPa. Gapswere successfully bridged with LTW by using a two-dimensional model to design theoperating parameters. To achieve higher modeling accuracy, a three-dimensional modelmight better simulate the thermal diffusion in the direction of laser travel.DOI: 10.1115/1.2769731

Keywords: laser welding, gap bridging, modeling, PVC

ackground

Laser transmission welding LTW is a popular thermoplasticoining option because it is a contact-free operation that createsxcellent quality welds. Due to a relatively large operating win-ow for variation in process parameters, including weld velocity,aser power, and clamping pressure, LTW is a robust joining pro-ess from a manufacturing viewpoint 13. One important pro-ess variable not previously explored in LTW is the presence ofaps in the joint.

Gaps occur in a joint for a variety of reasons including poorimensional control of mating part features, inadequate clampingorce, poor clamping location, warping, and poor joint design. Theresence of gaps in LTW using the contour method is a majoroncern because the process relies on thermal contact conductionetween the absorptive part and the transmissive part 2. Whenhese two parts are not in contact, conduction of the heat createdy laser radiation will not occur across the part interface, causinghe temperature of the absorptive part to rapidly increase. If thehermal expansion of the absorptive part does not create contactith the transmissive part and bridge the gap, thermal decom-osition of the absorptive part will likely occur.

Very little previous work has investigated bridging gaps inTW from either an experimental or a modeling approach. Russekt al. 4 briefly reports that bridging gaps is possible by increas-ng the optical penetration depth through changing the absorptionoefficient of absorbing material. This work states that gaps up to50 m are bridgeable using a circular laser spot in contour weld-ng 4. It should be noted that simultaneous and quasisimulta-

Contributed by the Manufacturing Engineering Division of ASME for publicationn the JOURNAL OF MANUFACTURING SCIENCE AND ENGINEERING. Manuscript receivedovember 3, 2006; final manuscript received July 6, 2007. Review conducted by Y.

awrence Yao.

ournal of Manufacturing Science and EngineeringCopyright 20

aded 28 Nov 2007 to 130.215.49.80. Redistribution subject to ASME

neous variants of LTW create meltdown at the joint. Bridginggaps is not as significant of a challenge with these two variants ofLTW as it is for the contour method.

Designing a laser transmission weld to bridge a gap requirescareful consideration of the heating distribution. The absorbingpart must be heated slowly to allow conduction into the bulk ofthe material, which will increase the thermal strain and allow thetwo parts to meet. Achieving the necessary thermal strain is nottrivial because the thermal conductivity of polymers is relativelylow and during a longer weld time, the possibility of thermaldecomposition becomes greater.

This paper presents an investigation of bridging gaps in LTW ofPVC using the contour method. Two different gap sizes will bediscussed, 12.7 m and 25.4 m. Using a numerical model pre-viously developed 2, simulations were run that design operatingparameters for both gap sizes. Using the designed operating pa-rameters, samples were welded and assessed for aesthetics, weldstrength, and weld width.

Laser Transmission Welding Model DescriptionA comprehensive numerical model was developed from first

principles of heat transfer and present in previous works 13.This model uses the energy balance method to calculate the tem-perature at nodes in two dimensions: into the material z directionand perpendicular to the direction of laser travel x direction. Themodel includes radiation from the material surfaces to the sur-roundings, convection from the external surfaces to the surround-ing air, laser reflection from both surfaces, heat generation withineach material from laser absorption, conduction within each ma-terial, and contact conduction between the two parts. A diagramexplaining the heat transfer aspects of the model can be seen inFig. 1.

In addition to calculating the temperature of each node, themodel also calculates the joining pressure at the interface between

the two parts. Initial clamping and thermal expansion during heat-

DECEMBER 2007, Vol. 129 / 101107 by ASME

license or copyright; see http://www.asme.org/terms/Terms_Use.cfm

igas

mGmctda

iAl

wctpdtcaHL

M

gTcrc1sapw

Ftmtel

1

Downlo

ng create this joining pressure. In the case of welding across aap, the initial joining pressure is zero and only begins to risefter sufficient thermal expansion creates contact between the ab-orptive and transmissive parts.

The model also includes many advanced attributes includingaterial properties that vary with temperature and pressure and aaussian laser distribution obtained from experimental measure-ents 1,2. Material properties that vary with temperature in-

lude the specific volume 5, which allows the thermal expansiono be calculated, the absorption coefficient 6, the elastic modulus7,8, the specific heat 8, and the thermal conductivity 8. Ad-itionally, the contact conduction varies with both temperaturend joining pressure and warrants further discussion.

Contact conduction between the joined parts is vital to LTW, ass demonstrated most emphatically when evaluating gap bridging.

model developed based on microscopic elastic deformation al-ows the contact conduction to be expressed as follows:

hc =1.49kmab

R 2.3P

Emab0.935 1

here hc is the contact conductance W/m2 K, k is the thermalonductivity W/m K, mab is the mean asperity slope rad, R ishe root mean square of the surface roughness m, P is the joiningressure Pa, and E is the elastic modulus Pa 9. This equationemonstrates that the pressure is nearly directly proportional tohe contact conduction; without pressure, conduction does not oc-ur. While it can be argued that convection and radiation do occurcross a gap, these are not significant compared to conduction.igh contact conduction is paramount to creating a successfulTW.

odeling Gap BridgingThe described model is used to simulate LTW for two different

ap sizes, 12.7 m and 25.4 m, using the same part geometry.hese gap sizes were selected as they sufficiently demonstrate thehanges in process parameters necessary to bridge a gap withineasonable welding velocities and can be easily constructed withommercially available shims. The example joint consists of two27 mm long25 mm wide3.2 mm thick PVC parts with aurface roughness of 1.3 m; the absorptive part is gray in colornd the transmissive part is clear. Both the clear and transparentarts are type I PVC from K-mac Plastics 1. The transmissive partill be placed above the gray part and fixtured such that a known

1

ig. 1 This diagram shows the heat transfer components ofhe two-dimensional numerical model. Material B is the trans-

issive part and Material C is the absorptive part. In this view,he laser beam is collinear with the positive z axis and is trav-ling into the paper in the direction of the positive y axis notabeled.

K-mac Plastic, 3821 Clay Ave. SW, Wyoming, MI 49548.

012 / Vol. 129, DECEMBER 2007

aded 28 Nov 2007 to 130.215.49.80. Redistribution subject to ASME

gap between the two parts is obtained. The radiation source is afiber coupled diode laser operating at a wavelength of 808 nmwith a maximum output power of 40 W.

The model is used in an iterative manner to achieve the desiredweld characteristics by varying the process parameters as previ-ously described 1,2. To provide a match to previous work, thelaser beam diameter is set to 5.7 mm. Through an iterative designprocess, the laser parameters selected to bridge a 12.7 m0.0005 in. gap have a laser velocity of 0.0025 m/s 0.10 in./ sand a laser power of 2.5 W. For reference, when operating with-out a gap, an applied clamping pressure of 2 MPa and a beamdiameter of 5.7 mm, the solution parameters were a weld velocityof 0.06 m/s and a laser power of 17 W, which created a 2.5 mmwide weld 1,2.

The resolution and computation speed of the model can bemodified by adjusting the distance between the nodes within thematerials, which changes the overall number of nodes, and bychanging the time step. In simulating the 12.7 m gap, the modelis run for 2.3 s with a time step of 2 ms. The distance betweeneach node is set to 0.05 mm. Selecting the time step and distancebetween nodes is a balance between processing time and accuracywhile satisfying the stability criterion,

=kt

Cx2

1

22

where is the mesh Fourier number, t is the time step, is themass density, C is the specific heat, and x is the distance be-tween nodes 10. Output plots from the model for this designsolution are presented in Figs. 2 and 3.

As can be seen in Fig. 2, a large amount of time elapses beforethe gap is closed and heating of the transmissive material begins.Even with a very low laser power of 2.5 W, the temperaturewithin the absorptive material reaches over 786 K, which causesconcern of thermal decomposition. The weld width predicted bythe model is the width that exceeds a temperature of 485 K, whichis most easily observed in the lower plot of Fig. 3. 485 K is set asthe defining temperature of a weld from previous work weldingPVC sheets with a heated pin 1,11. The predicted weld width forthis set of process parameters is 2.10 mm, markedly narrower thanthe 2.50 mm wide weld obtained when no gap was present and thelaser beam was the same diameter.

Process parameters were also designed for a larger gap size of25.4 m 0.001 in. As expected, a slower weld velocity is re-quired to allow sufficient thermal expansion to bridge the largergap. To avoid decomposing the polymer during longer weld times,the line energy, defined as the laser power divided by the laservelocity, needs to be decreased. The line energy is decreased byeither decreasing the laser power or increasing the laser beamdiameter. Below 2.5 W of power, the available diode laser signifi-cantly loses efficiency and the output power is more difficult topredict 12. For this reason, an additional constraint added to thisdesign is a desire to operate at or above 2.5 W. Using an iterativedesign method, suitable solution was found at the following oper-ating parameters: a laser power of 2.5 W, a beam diameter of8 mm, and a weld velocity of 0.001 m/s 0.039 in./ s. Using atime step of 0.01 s and a distance between the nodes of 0.1 mm,the model produced the plots found in Figs. 4 and 5. The time stepand distance between the nodes were increased from the earliermodel to keep the processing manageable during the 9 s weldtime.

It should be noted that welding across a significant gap requiresa very slow welding velocity. This low velocity is needed to el-evate the temperature through a considerable depth in the absorp-tive part, creating the needed thermal expansion to bridge the gap.This heating away from the weld zone can especially be observedin Fig. 5 where the temperature contour lines extend a significant

distance in the depth direction from the part interface. The weld

Transactions of the ASME

license or copyright; see http://www.asme.org/terms/Terms_Use.cfm

wwl

E

ctisttt

ans

J

Downlo

idth for this solution is 3.00 mm and again is defined as theidth above 485 K. This larger width is primarily due to the

arger laser beam diameter of 8 mm.

xperimental SetupModeling gap bridging with LTW has not been previously ac-

omplished and thus the described model needs to be experimen-ally validated. A method was designed to create a known gap sizen a T-joint geometry in a welding fixture. To create a known gapize, two short pieces of polyester shimstock are placed on top ofhe absorptive part at both ends outside of the weld zone. Theransmissive part is then placed horizontally on the shims, creating

Fig. 2 The four output subplots of the modelSubplot a shows the temperature of the transas a function of time and width. Subplot b isthe time step that the maximum temperature=3.2103 m. Subplot c shows the internal psubplot d shows the gap size along the widalong the x axis Fig. 1 with a mirror boundabefore the gap is closed and heating of the tr

he T-joint geometry with a known gap between the two parts, as

ournal of Manufacturing Science and Engineering

aded 28 Nov 2007 to 130.215.49.80. Redistribution subject to ASME

seen in Fig. 6. The assembled samples are placed in the weldingfixture Fig. 7 to secure the T-joint geometry and assure align-ment with the laser during welding. A very minimal pressure of50 kPa was applied to the sample to maintain contact from thetransmissive part to the shims and from the shims to the absorp-tive part.

The laser system used for the welding experiments consists of a30 W, 808 nm diode laser bar manufactured by Cutting Edge Op-tronics that is conductively cooled using a Peltier cooler. The di-ode bar is coupled to a 2 m long, 1.1 mm diameter fiber opticcable with an output lens assembly that is kept clear of dust anddebris by a positive airflow nozzle. The laser spot diameter is

the design solution bridging a 12.7 m gap.ssive part at the interface of the two materialszoomed contour plot of the interface zone atcurs. In this case, the interface is at a depthsure as a function of time and width. Finally,s a function of time. The width dimension iscondition at x=0. Note the large elapse timemissive material begins.

formia

ocres

th ary

adjustable between 2 mm and 10 mm by moving a slide that

DECEMBER 2007, Vol. 129 / 1013

license or copy...